Surface stress effects on the bending properties of fcc metal nanowires


 Bertram Simon
 2 years ago
 Views:
Transcription
1 PHYSICAL REVIEW B 79, Surface stress effects on the bending properties of fcc metal nanowires Geng Yun and Harold S. Park* Department of Mechanical Engineering, University of Colorado, Boulder, Colorado 839, USA Received November 28; revised manuscript received 24 March 29; published 9 May 29 The major purpose of this work is to investigate surface stress effects on the bending behavior and properties of / gold nanowires with both fixed/fixed and fixed/free boundary conditions. The results are obtained through utilization of the recently developed surface CauchyBorn model, which captures surface stress effects on the elastic properties of nanostructures through a threedimensional, nonlinear finite element formulation. There are several interesting findings in the present work. First, we quantify the stress and displacement fields that result in the nanowires due to bending deformation. In doing so, we find that regardless of boundary condition, the stresses that are present in the nanowires due to deformation induced by surface stresses prior to any applied bending deformation dominate any stresses that are generated by the bending deformation unless very large 5% bending strains are applied. In contrast, when the stresses and displacements induced by surface stresses prior to bending are subtracted from the stress and displacement fields of the bent nanowires, we find that the bending stresses and displacements do match the solutions expected from bulk continuum beam theory, but only within the nanowire bulk, and not at the nanowire surfaces. Second, we find that the deformation induced by surface stresses also has a significant impact on the nanowire Young s modulus that is extracted from the bending simulations, where a strong boundarycondition dependence is also found. By comparing all results to those that would be obtained using various linear surfaceelastic theories, we demonstrate that a nonlinear, finite deformation formulation that captures changes in both bulk and surfaceelastic properties resulting from surface stressinduced deformation is critical to reproducing the experimentally observed boundarycondition dependence in Young s modulus of metal nanowires. Furthermore, we demonstrate that linear surfaceelastic theories based solely on the surface energy erroneously predict an increase in Young s modulus with decreasing nanowire size regardless of boundary condition. In contrast, while the linear surfaceelastic theories based upon the Gurtin and Murdoch formalism can theoretically predict elastic softening with decreasing size, we demonstrate that, regardless of boundary condition, the stiffening due to the surface stress dominates the softening due to the surface stiffness for the range of nanowire geometries considered in the present work. Finally, we determine that the nanowire Young s modulus is essentially identical when calculated via either bending or resonance for both boundary conditions, indicating that surface effects have a similar impact on the elastic properties of nanowires for both loading conditions. DOI:.3/PhysRevB PACS number s : w, g, Gy, k I. INTRODUCTION Nanowires have been intensely researched by both the scientific and engineering communities over the past decade. 3 One of the major reasons for the surge in interest for nanowires has been due to their potential as the basic building block for nanoelectromechanical systems NEMS. As the basic building block for NEMS, nanowires will be used to perform chemical sensing, act as highfrequency oscillators, used to perform ultrasensitive mass and force detection, and to act as next generation wireless components. 4 6 Of relevance to the present study, in many NEMS applications, nanowires will be synthesized and actuated in beamlike geometries and configurations that appear amenable to description using standard continuum beam theory. Due to the fact that nanowires have beamlike geometries and because many of the potential NEMS applications require knowledge of the nanowire elastic properties, there has been a recent surge of interest in both experimental and theoretical techniques to characterize the elastic properties of nanowires. The experimental characterization has typically involved two distinct experimental techniques, those utilizing atomic force microscope AFM induced bending, 7 4 and those utilizing resonancebased measurements. 5 2 Unfortunately, there is significant scatter in the experimental results, 3 with some reporting an enhanced elastic stiffness,,,8 some reporting a reduced elastic stiffness, 7,2 23 and some reporting no variation in elastic stiffness 8,9,3,4 with decreasing nanostructure size. We note that the crosssectional sizes of these nanowires typically are in the range of 5 25 nm, where nanoscale size and surface effects may be limited. The size dependence in elastic behavior and properties at the nanoscale arises due to surface stress and surfaceelastic effects, 28 3 both of which occur due to the reduced coordination number 3 that characterizes surface atoms as compared to those that lie within the material bulk. Furthermore, the percentage of surface atoms, and therefore the percentage of atoms that have a reduced coordination number increases with the increasing surface area to volume ratio that is characteristic of nanomaterials. Because the surface effects are related to surface area to volume ratio, the surface stress and surfaceelastic effects become significant with decreasing structural size. Atomistic modeling has predicted a strong size dependence in the elastic properties of nanostructures at crosssectional sizes smaller than about nm. 28,29,32 35 However, most atomistic calculations have been performed considering 982/29/79 9 / The American Physical Society
2 GENG YUN AND HAROLD S. PARK PHYSICAL REVIEW B 79, axial tensile loading, while comparably few results exist for bending This fact is critical because as is well known, the surfaces of beams are subject to the maximum tensile and compressive states of stress under bending. Because surfaces are the key factor in altering the elastic properties of nanostructures, it is likely that the elastic properties of nanowires measured under bending may differ from those measured under resonance or axial testing approaches. 39 The theoretical models that have been developed for nanostructures are typically based upon further developments of the linear surfaceelastic theory of Gurtin and Murdoch, 4 which treats the surface as a deformable elastic medium attached to the bulk and which can be described using a Hooke slawtype linear elastic stress strain relationship. Various surfaceelastic models have been developed 3,39,4 46 and utilized to study the effects of surfaces on the bending behavior and properties of nanowires. There are several key shortcomings of these models that have motivated the present work. In particular, the models are generally twodimensional 2D, which neglects the changes in crosssectional area that arise due to the deformation induced by surface stresses, some models assume that surface physics can be captured using overly simplistic interatomic pair potentials to describe the surface bond energetics; these are physically incorrect because pair potentials predict that the surface stress of metals is compressive rather than tensile, 3 the complex nature of the analytic equations makes these models difficult to implement in finite element FE type numerical analysis, 4 due to equilibrium requirements enforced between the bulk and surface in deriving the surfaceelastic formulation, 24,4 the surface stress in the surfaceelastic formulation is a 2 2 inplane stress tensor, where the outofplane stress component must be zero to satisfy the mechanical equilibrium condition. The implication of this 2 2 inplane surface stress tensor is that surfaceelastic formulations are unable to capture the surfacestressdriven compressive relaxation that metal nanowires are known to undergo Due to the linear elastic constitutive response that is assumed for both the bulk and surface, the surfaceelastic models are unable to capture the nonlinear elasticity of the nanowire bulk which results due to surface stress driven compressive strain, and which is known to play a critical role in the elastic properties of metal nanowires, 29 6 The stress and displacement fields in the nanowires have not been quantified to date for different boundary conditions while accounting for surface stressinduced deformation using a nonlinear, finite deformation constitutive model. In the present work, we utilize the recently developed surface CauchyBorn SCB model, 47,48 which captures the bulk and surfaceelastic properties of nanostructures directly from an underlying atomistic potential 49,5 using nonlinear, finite deformation kinematics to study surface stress effects on the bending behavior and properties of gold nanowires with transverse surfaces. We focus upon intermediatesize nanowires, with crosssectional dimensions between 5 and 25 nm, in order to bridge the small size scales that have been studied atomistically, and the larger sizes that have been evaluated experimentally. By considering nanowires of varying crosssectional area and aspect ratio, using both fixed/free and fixed/fixed boundary conditions, we arrive at the key findings of the present work, which are: corresponding to the discussion above regarding the inability of current surfaceelastic formulations to capture surfacestressdriven relaxation of the nanowires, we find that the stresses and displacements induced in the nanowires due to surfacestressdriven relaxation are significantly larger than the stresses and displacements induced by bending of the nanowires, even out to large % bending strains and for fairly large nanowire cross sections 25 nm. 2 The bending stiffness, and therefore Young s modulus of the nanowires is strongly boundary condition and size dependent. We discuss the implications of these findings, and compare our results to previous analytic results based upon linear surface elasticity for nanowire bending,,42 to demonstrate how and why our findings are different from those found using either linear continuum beam theory or linear surfaceelasticity theory. Finally, we compare results for the nanowire Young s modulus obtained via bending in the present work to resonance 5 to determine if there are any quantifiable differences induced by the testing or loading method in how surfaces impact the nanowire Young s modulus. II. SURFACE CAUCHYBORN MODEL A. Overview The standard bulk CauchyBorn BCB model is a multiscale, finite deformation constitutive model that enables the calculation of continuum stress and stiffness directly from an underlying interatomic potential energy However, because the BCB model does not account for critical nanoscale surface stress effects, the SCB model was recently developed by Park et al. 47,48,55 to capture surface stress effects within the framework of the CauchyBorn approximation. Because the SCB formulation for FCC metals was presented in previous works by Park et al., 48,5 we refer the interested reader to those works for a detailed exposition on the SCB model. As noted in previous expositions on the SCB model for FCC metals, 48,5 the SCB model is based on constructing a surface strain energy density C of a representative surface unit cell, where C=F T F is the continuum stretch tensor, indicating that the SCB model is a nonlinear, finite deformation model. The surface energy density C is calculated in the present work using the embedded atom EAM potential for gold of Foiles. 5 We note that extensive studies comparing the SCB model and purely atomistic simulations for the surfacestressdriven relaxation of fixed/free FCC metal nanowires have been performed using EAM potentials by Park and Klein; 48 the accuracy of the SCB model in predicting the compressive relaxation strain of the free end was found to be less than % for nanowire crosssectional sizes larger than about 8 nm. We also note that the EAM potentials utilized in the present work are well known to underestimate both the surface energy and surface stress by 3 5 % as compared to DFT calculations or experiments; 58 these errors are transferred to the SCB model because it is based upon the EAM potentials. We also emphasize the differences between the SCB formulation for surface stress and surface energy, and the tradi
3 SURFACE STRESS EFFECTS ON THE BENDING tional thermodynamic definition of surface stress see for example 24,59, = + C, where is the surface stress, is the residual strainindependent portion of the surface stress, C is the surfaceelastic straindependent part of the surface stress, and where C is the constant surfaceelastic stiffness. Interestingly, recent works by Park and Klein 5 and Park 6 have demonstrated that if finite deformation kinematics is considered, as they are in the SCB model, the residual surface stress does in fact contribute significantly to the resonant frequencies of both metallic and semiconducting nanowires. The difference is that the SCB surface energy density C represents the actual surface energy of the surface unit cell, and not the excess in energy as compared to a representative bulk atom, which is how the surface energy is traditionally defined thermodynamically. 24 Once the surface energy density is known, the second surface PiolaKirchoff stress and the surface stiffness can be calculated by taking derivatives of the surface energy density C with respect to the stretch tensor C see Eq. 2 in Park and Klein 48. III. NUMERICAL EXAMPLES All numerical examples were performed on threedimensional, singlecrystal gold nanowires of length L and TABLE I. Summary of nanowire geometries considered: constant aspect ratio, and constant crosssectional area. All dimensions are in Angstroms Å. CAR PHYSICAL REVIEW B 79, CCSA square cross section of width a. Two different parametric studies are conducted in this work, which consider nanowires with constant crosssectional area CCSA, where a =6 Å, and constant aspect ratio CAR of L/a=8; the geometries are summarized in Table I. All simulations were performed using the Sandiadeveloped simulation code Tahoe. 6 All wires had a longitudinal orientation with transverse surfaces, while two different boundary conditions, fixed/free and fixed/fixed ends were used; we note that these boundary conditions are similar to what has been assumed in both experimental,,4 studies and theoretical, studies of nanowire bending, to which we will compare the obtained SCB results in Sec. VI. All finite element FE simulations were performed using the stated boundary conditions and utilized regular meshes of eightnode hexahedral elements, Relaxed Stress of Fixed/Fixed SCB Nanowires at X=5L/8 5 Relaxed Stress of Fixed/Fixed SCB Nanowires at X=5L/ x5x5 44x8x8 68x2x2 92x24x x5x5 44x8x8 68x2x2 92x24x σ (ev/angstroms 3 ) x σ 2 (ev/angstroms 3 ) x 4 Relaxed Displacement of Fixed/Fixed SCB Nanowires at X=5L/8 5 2x5x5 44x8x8 68x2x2 92x24x (c) Y Displacement (Angstroms) FIG.. Color online Stresses and y displacements in CAR fixed/fixed nanowires after deformation due to surface stresses
4 GENG YUN AND HAROLD S. PARK PHYSICAL REVIEW B 79, Bending Stress of Fixed/Fixed BCB Nanowires at X=5L/8 5 2x5x5 44x8x8 68x2x2 92x24x24 Bending Stress of Fixed/Fixed SCB Nanowires at X=5L/ x5x5 44x8x8 68x2x2 92x24x σ (ev/angstroms 3 ) x σ (ev/angstroms 3 ) x 3 FIG. 2. Color online Bending for BCB and SCB CAR fixed/fixed nanowires. with at least ten finite elements through the nanowire thickness. Regardless of whether fixed/free or fixed/fixed boundary conditions are utilized, the nanowires are initially out of equilibrium due to the surface stresses. Therefore, before any external bending deformation was applied, we first determined the minimum energy, or relaxed configurations of the nanowires due to the surface stresses. Finding the minimumenergy configurations corresponds directly to what would occur experimentally, in which the nanowires deform in response to surface stresses after the synthesis or etching process. Once the minimumenergy configuration due to surface stresses was determined, external loading was applied incrementally under quasistatic loading, such that the nanowire could equilibrate due to a given load increment before additional loading was applied. The elastic properties and the bending stresses were determined after applying bending strains of 8.5e3% for the CAR nanowires and 8.6e2% for the CCSA nanowires; however, additional calculations were carried out where the nanowires were bent to strains nearing 5%. In all cases, we also performed the simulations using the BCB model, i.e., without surface stresses, to quantify how surface stresses cause variations in both the nanowire elastic properties, as well as the stress and displacement fields, as a function of size. IV. STRESS AND DISPLACEMENT FIELD IN THE NANOWIRE AFTER SURFACE STRESS INDUCED DEFORMATION Before discussing the bendinginduced stresses and displacements in the nanowires, we first discuss the state of stress and the displacement fields that occur in the nanowires as a result of surface stressinduced deformation, i.e., in the absence of any applied external forces, as we will demonstrate that this is critical to the understanding of nanowire bending stresses, deformation, and elastic properties. As discussed earlier, the nanowires are initially out of equilibrium due to the surface stresses, and therefore deform in response to the surface stresses until an equilibrium configuration is reached in which the tensile surface stresses are balanced by compressive stresses within the nanowire bulk. While both fixed/fixed and fixed/free CCSA and CAR nanowires were considered, we focus on the fixed/fixed CAR nanowires as the other geometries and boundary conditions Bending Stress of Fixed/Fixed BCB Nanowires at X=5L/8 5 2x5x5 44x8x8 68x2x2 92x24x24 Bending Stress of Fixed/Fixed SCB Nanowires at X=5L/ x5x5 44x8x8 68x2x2 92x24x σ (ev/angstroms 3 ) 2 x σ (ev/angstroms 3 ) 2 x 4 FIG. 3. Color online Bending 2 for BCB and SCB CAR fixed/fixed nanowires
5 SURFACE STRESS EFFECTS ON THE BENDING PHYSICAL REVIEW B 79, Bending Displacement of Fixed/Fixed BCB Nanowires at X=5L/ x5x5 44x8x8 68x2x2 92x24x Y Displacement (Angstroms) Bending Displacement of Fixed/Fixed SCB Nanowires at X=5L/8 5 2x5x5 44x8x8 68x2x2 92x24x Y Displacement (Angstroms) FIG. 4. Color online Bending y displacement across the cross section for fixed/fixed CAR nanowires after bending force has been applied for both BCB and SCB nanowires. lead to similar conclusions regarding surface stress effects on the displacements and stresses in the nanowires. The stresses in the fixed/fixed CAR nanowires after surfacestressdriven relaxation are shown in Fig.. For the normal stress,we first note that is positive at the nanowire surfaces but negative within the nanowire core. The normal stress is positive at the free surfaces of the nanowire due to the tensile nature of metallic surface stresses. 58 In general, is larger at the surfaces for fixed/fixed nanowires due to the fact that the fixed/free nanowires can contract axially and thereby relieve some of the effects of the tensile surface stress. In contrast, is negative within the nanowire bulk for both boundary conditions; it is negative for the fixed/fixed case because while both ends of the nanowire are fixed, the interior still relaxes and compresses slightly in response to the surface stresses. The sizedependent effect of the surface stresses reveals itself in the normal stresses in Fig.. For the fixed/fixed CAR nanowires in Fig., there is a slight difference in between the largest nanowire with crosssectional length 24 nm, and the smallest, with crosssectional length of 5 nm; =.2 ev/å 3 for the 24 nm CAR nanowire, while =.6 ev/a 3, or about.25 GPa, for the 5 nm CAR nanowire. While the fixed ends prevent the nanowire from contracting along its length, the smaller 5 nm CAR nanowire experiences slightly more bulk compression due to surface stresses, and thus is subject to a larger compressive. In contrast to the normal stress, the shear stress 2 = in the interior of the nanowires, regardless of the boundary condition. On the surfaces of the nanowires, the nature of the shear stress depends upon the state of surface deformation; 2 is positive in Fig. at the surfaces because the surfaces are in tension resulting from the fixed end boundary conditions. Regarding the displacement field, for the fixed/fixed nanowire in Fig., we note that the vertical y displacements are negative at the top surface and positive at the bottom surface, indicating that the crosssectional area has contracted in response to the surface stresses. Before moving forward to discuss the effects of bending forces on the nanowire state of stress, we reemphasize that the results shown in Fig. constitute the state of stress and the vertical y displacement field in the nanowires before any externally applied forces to induced bending are applied. V. NANOWIRE BENDING STRESS AND DISPLACEMENT RESULTS We now discuss the actual bending stresses and displacements for the CAR nanowires, for both fixed/fixed and fixed/ free boundary conditions. Again, we emphasize that the bending forces were applied after the nanowires were allowed to find a minimumenergy configuration due to the surface stresses, as was discussed in the previous section. We show results for both SCB and BCB i.e., without surface stress effects CAR nanowires to compare how the bending stresses of nanowires are different when surface stresses are accounted for. The stress in the nanowire after bending for the fixed/ fixed BCB and SCB CAR nanowires is shown in Figs. 2 and 3. As can be seen, the BCB nanowire stresses exhibit the expected trends from continuum beam theory, i.e., is linear, as seen in Fig. 2, and 2 is parabolic, as seen in Fig. 3. However, the bending stresses for the SCB nanowire are quite different. As seen in Figs. 2 and 3, the normal stress does not exhibit a linear pattern, nor does the shear stress 2 exhibit a parabolic pattern. In fact, the bending stresses for the SCB nanowires appear to be remarkably similar to the stresses present in the nanowires due to surfacestressinduced deformation as previously seen in Fig. for fixed/ fixed CAR nanowires. Similarly, a comparison between the ydisplacement field after bending at the center of the fixed/fixed beam for SCB and BCB nanowires is shown in Fig. 4. While the BCB displacement field is parabolic, and slightly negative due to the applied force, the displacement field in the SCB nanowire is significantly different. There, the top surface has a significantly larger downward displacement than the bottom surface, and there is an oscillation of the displacement field between the two surfaces. Furthermore, the SCB displacement field in Fig. 4 appears as though it can be obtained by
6 GENG YUN AND HAROLD S. PARK PHYSICAL REVIEW B 79, Fixed/Fixed 2x5x5 Nanowires at X=5L/8 8 Fixed/Fixed 2x5x5 Nanowires at X=5L/8 6 4 BCB SCB Minus Relaxation Stress 6 4 BCB SCB Minus Relaxation Stress σ (ev/angstroms 3 ) x σ (ev/angstroms 3 ) 2 x 7 8 Fixed/Fixed 2x5x5 Nanowires at X=5L/ BCB SCB Minus Relaxation Displacement (c) Y Displacement (Angstroms) FIG. 5. Bending stresses and y displacement across the cross section for CAR nanowires after relaxation stress and displacement in Fig. has been subtracted from SCB bending results in Figs adding the relaxed SCB displacement field in Fig. and the BCB bending displacement field in Fig. 4. Due to the similarity between the bending stresses in Figs. 2 and 3, and the relaxed stresses i.e., the stresses due to deformation induced by surface stresses before the application of any external bending forces in Fig., and also between the bending displacements in Fig. 4 and the relaxed displacements in Fig., we plot in Fig. 5 the stresses and displacements in the SCB nanowire after subtracting the relaxed stresses and displacements. As can be observed, once the relaxed stresses and displacements are removed, the SCB nanowire exhibits bending stresses and displacements similar to those expected from continuum beam theory, and exhibited by the BCB nanowire: exhibits a largely linear pattern within the nanowire bulk, with deviation occurring near the nanowire surfaces, 2 exhibits the expected parabolic pattern, again matching the BCB solution within the nanowire bulk, and deviating near the surface, while the bending displacements again match closely, with the displacement error being about.3%. Furthermore, we note that the normal stress is more positive at the bottom of the fixed/fixed nanowire than at the top; this makes sense as the top surface of beams are in compression for bending in a fixed/fixed configuration, while the bottom of the same beam is under tension. We conclude this section on the nanowire bending stresses and displacements with three comments. First, our results demonstrate that the nanowire bending stresses and displacements are strongly impacted by the residual stress and displacement fields that are present in the nanowire due to surface stress driven relaxation; these results are expected to be quantitatively valid as they were obtained using EAM potentials 5 that are known to underestimate the surface stress by 3 5 % as compared to DFT calculations. 58 Prior works have focused upon predicting size and surface effects on the bending stiffness of the nanowires; 3,39,4 45 we will demonstrate in the next section that, just as deformation induced by surface stresses has a significant effect on the nanowire bending stresses and displacements, the deformation induced by surface stresses also has a significant effect on the elastic properties of the nanowires. Second, we have demonstrated that the bending stresses and displacements, when the relaxed stresses and displacements due to deformation induced by surface stresses are removed, do follow the expected continuum beam theory solutions, i.e., linear for the normal stress and parabolic for the shear stress 2, but only within the nanowire bulk.at the surfaces, the normal and shear stresses deviate substantially, with dependencies on the boundary condition and the
7 SURFACE STRESS EFFECTS ON THE BENDING PHYSICAL REVIEW B 79, Force (ev/angstroms) Fixed/fixed Constant Cross Sectional Area Nanowires 8 BCB, L=28 nm 7 SCB, L=28 nm BCB, L=256 nm 6 SCB, L=256 nm BCB, L=48 nm 5 SCB, L=48 nm Force (ev/angstroms) Fixed/free Constant Cross Sectional Area Nanowires BCB, L=28 nm SCB, L=28 nm BCB, L=256 nm SCB, L=256 nm BCB, L=48 nm SCB, L=48 nm Displacement (Angstroms) Displacement (Angstroms) FIG. 6. Color online Force versus displacement relationship for CCSA nanowires. resulting state of deformation due to surface stress driven relaxation. Finally, we have performed additional simulations which have demonstrated that it is only for very large bending strains, i.e., 5%, where the stresses induced by bending become larger than the stresses induced by surface stress driven relaxation, and only then for fixed/fixed, and not fixed/free nanowires. Because of this factor, and because the bending of the nanowires is likely to occur over much smaller bending strains, the present results are strongly indicative that continuum beam theory solutions cannot be utilized to describe the bending stress state in nanowires that are subject to deformation due to surface stresses. VI. NANOWIRE ELASTIC PROPERTIES FROM BENDING SIMULATIONS The second objective of this work is to characterize the boundaryconditiondependent elastic properties of the nanowires as obtained using the finite element method FEM calculations and both the BCB and SCB models; the BCB results are pertinent as they enable us to quantify the effects of surface stresses on the nanowire elastic properties for each geometry considered. To do so, we first show the force vs displacement relationships obtained for the various nanowire geometries and boundary conditions. The force vs displacement relationship is important as it is the quantity that is extracted during experimental measurements of nanowire bending. 8,9,,2,4 Through calculation or measurement of the force vs displacement curve, the bending stiffness k of the nanowires can be directly calculated from F = k d, 2 where d is the increment in bending displacement that results from the increment in applied force F, and k is the spring constantlike stiffness that relates the force and displacement. The bending stiffness k is also a critical parameter because it enables experimentalists to, using the assumptions of linear elastic continuum beam theory, estimate the nanowire Young s modulus E using known solutions for fixed/fixed and fixed/free beams, where the stiffness k=92ei/l 3 for a fixed/fixed beam loaded at the beam center, and k=3ei/l 3 for a fixed/free beam loaded at the free end. We first discuss the results for the elastic properties of CCSA nanowires, where the force vs displacement relationships for fixed/fixed and fixed/free boundary conditions are shown in Fig. 6, and where the calculated bulknormalized bending stiffness k and Young s modulus E for both boundary conditions and all geometries are summarized in Table II. In analyzing Fig. 6, it is evident that the boundary conditions play a substantial role in the force vs displacement response, and therefore the elastic properties of the nanowires. For the fixed/fixed CCSA nanowires, for all nanowire lengths, more force is required to deform the SCB nanowires to the same displacement as compared to the BCB nanowires of the same size. In contrast, for the fixed/free CCSA nanowires, the force vs displacement plots for the SCB and BCB nanowires are nearly indistinguishable. The disparities in the force vs displacement response for the two boundary conditions for the CCSA nanowires are highlighted in Table II, where the bulknormalized bending stiffnesses, and thus Young s modulus for the boundary conditions show very different results. First, Table II demonstrates that Young s modulus for the SCB nanowires shows a slightly decreasing trend with increasing aspect ratio, where the modulus of the fixed/free SCB nanowire is approximately 98% of the bending modulus of the BCB nanowire TABLE II. Normalized stiffness and Young s modulus, both expressed as a ratio of SCB/BCB, for CCSA nanowires. Geometry k scb k bcb = E scb E bcb fixed/free k scb k bcb = E scb E bcb fixed/fixed
8 GENG YUN AND HAROLD S. PARK PHYSICAL REVIEW B 79, Force (ev/angstroms) Fixed/fixed Constant Aspect Ratio Nanowires BCB (All) SCB, L=2 nm SCB, L=68 nm SCB, L=92 nm Force (ev/angstroms) 3.5 x Fixed/free Constant Aspect Ratio Nanowires BCB (All) SCB, L=2 nm SCB, L=68 nm SCB, L=92 nm Displacement (Angstroms) Displacement (Angstroms) FIG. 7. Color online Force versus displacement relationship for CAR nanowires. when the aspect ratio L/a=3. The nearly bulk or slightly softened elastic response of fixed/free metal nanowires has been observed both experimentally, 2 23 and using MD simulations. 36 However, the bending modulus ratio for fixed/fixed nanowires shows a markedly different trend. In particular, the bending modulus for the SCB nanowires increases dramatically as compared to the BCB bending modulus with increasing aspect ratio, with a value more than 2.5 times the BCB value when the aspect ratio L/a=3. Similar increases in Young s modulus for fixed/fixed metal nanowires under bending have been found recently by multiple researchers;, we further discuss our results in comparison with analytic solutions for Young s modulus that include surface effects from both of those works, in the next section. To determine how the variations in the nanowire bending modulus scale with size, we also present the results for the CAR nanowires, which are summarized in Fig. 7 and Table III. The trends for the fixed/free boundary conditions are similar to that observed for the CCSA nanowires, where the force vs displacement response for the SCB and BCB nanowires are nearly indistinguishable. However, again, the SCB nanowires are observed in Fig. 7 to be elastically stiffer than the BCB nanowires of the same size for the fixed/fixed boundary conditions. Similarly, the bending modulus of the fixed/free SCB nanowires, as shown in Table III, are shown to be nearly indistinguishable from the bending modulus of the BCB nanowires; for all CAR geometries, the SCB bending modulus is only % smaller than the BCB bending modulus. In TABLE III. Normalized stiffness and Young s modulus, both expressed as a ratio of SCB/BCB, for CAR nanowires. Geometry k scb k bcb = E scb E bcb fixed/free k scb k bcb = E scb E bcb fixed/fixed contrast, the bending modulus of the fixed/fixed SCB nanowires is considerably elevated as compared to the fixed/fixed BCB nanowires. However, Table III also shows the manifestation of how surface effects impact the nanowires with varying size for the CAR nanowires; as the crosssectional size of the nanowires is increased, the divergence between the SCB and BCB bending moduli begins to diminish, which is expected due to the decrease in overall surface area to volume with increasing nanowire size. A. Discussion: Comparison to linear surfaceelastic models that account for surface stress and surface stiffness We now discuss reasons for the disparity in boundarycondition effects on the nanowire bending stiffness and Young s modulus. For fixed/fixed silver and lead nanowires, similar increases in both the bending stiffness and Young s modulus have been observed experimentally by multiple researchers., However, we note that the silver and lead nanowires were likely not ideal, defectfree single crystals, and did not have axial orientations or transverse surface orientations; for example, the silver nanowires considered by Jing et al. were covered with a native oxide layer. This is in contrast to the ideal, defectfree single crystal / gold nanowires that were studied in this work using the SCB model. To shed insights into the strengths and limitations of available analytic surfaceelastic solutions, we compare the SCB simulation results against those of Jing et al., who used the surfaceelastic formulation of Gurtin and Murdoch, 4 which accounts for both surface stress and surface stiffness C, to compare against their experimentally obtained bending stiffness of fixed/fixed silver nanowires. Taking Eq. 7 from Jing et al., and modifying the geometric parameters to account for the fact that our nanowires have a square, and not circular cross section, we obtain an expression for the bulknormalized Young s modulus as E eff =+ 8C L2 E fixed/fixed Ea 5Ea 3, 3 where E eff is the effective Young s modulus that accounts for surface effects, L is the nanowire length, E is the bulk
9 SURFACE STRESS EFFECTS ON THE BENDING PHYSICAL REVIEW B 79, k surf /k bulk Bending Stiffness of Fixed/Fixed CAR Nanowires SCB Jing:No ν,+c Jing:ν, C k surf /k bulk Bending Stiffness of Fixed/Fixed CCSA Nanowires, a=6 nm 4 SCB Jing:No ν,+c 3.5 Jing:ν, C FIG. 8. Color online Bulk normalized bending stiffness for fixed/fixed SCB CAR=8 and CCSA nanowires as compared to analytic surfaceelastic solutions of Jing et al. Ref. rewritten in Eq. 3. Young s modulus, and a is the nanowire crosssectional length. Because Jing et al. only studied the bending of fixed/ fixed nanowires, they did not derive an analytic solution for the effective Young s modulus of fixed/free nanowires. To compare the SCB fixed/free results against the Jing solution, we derive the Jing solution for fixed/free beams in the Appendix, while stating the final result here to be E eff =+ 8C L2 E fixed/free Ea 5Ea 3. 4 For Eqs. 3 and 4, the parameters utilized were E =36 GPa for gold, 5 =.98 ev/å 2, 5 and C =.329 ev/å 2 Ref. 59 ; both the surface stress and surface stiffness C are for gold surfaces, and constitute relaxed values. We additionally note that, unlike the original Jing model, we have accounted for transverse deformation effects by including dependence upon Poisson s ratio in Eqs. 3 and 4, where =.44 for bulk gold. Due to the geometric factor L 2 /a 3 that is present in Eqs. 3 and 4, we plot in Fig. 8 the bulknormalized bending stiffness or equivalently the bulknormalized bending modulus for the fixed/fixed nanowires as obtained using the SCB and two different Jing models against L 2 /a 3, where two different Jing models were considered for reasons now described. The Jing: no, +C curve in Fig. 8 represents the Jing solution as presented in Eq. 7 of Jing et al.; we refer to it in the discussion below as the original Jing model. In that work, transverse deformation was neglected, thus no dependence on Poisson s ratio was obtained. Furthermore, shear deformation was neglected in the Jing model by assuming that the nanowires had an aspect ratio that exceeded 6. Finally, the surface stiffness C was taken to be positive in the Jing work; this is in contrast to recent atomistic calculations which have shown that C should in fact be negative for most clean FCC metal surfaces, 59,62 as well as for incoherent FCC metalmetal interfaces, 62 though we note that the silver nanowires considered in the Jing models and experiments were enclosed by an oxide layer. The Jing:, C curve in Fig. 8 represents the solution of Eq. 3, where transverse deformation is accounted for, and where the surface stiffness C is taken to be negative, with values from Shenoy 59 for gold surfaces. We refer to this as the modified Jing model in the discussion below. We first observe that while the original Jing model gives reasonable agreement with the SCB results for the CAR= 8 nanowires in Fig. 8, the results differ significantly from the SCB results for the CCSA nanowires in Fig. 8. However, if transverse deformation is accounted for and the surface stiffness C is taken to be negative, the modified Jing model agrees very well with the SCB results for the CCSA nanowires in Fig. 8, with improved agreement with increasing aspect ratio, or increasing L 2 /a 3. In contrast, the agreement between the modified Jing model and the SCB results for the CAR= 8 geometries is not as good, for reasons discussed below. The fact that the SCB and modified Jing model have the least accuracy for the smallest aspect ratios is manifested for both small L 2 /a 3 for the CCSA nanowires, and also in Fig. 8 for the CAR= 8 nanowires. However, because of the improved agreement between the SCB and modified Jing model for the CCSA nanowires with increasing aspect ratio, we also calculated results in Fig. 9 for fixed/fixed CAR nanowires where the aspect ratio was 6 and 24, rather than 8 as seen in Fig. 8; the square crosssectional length a was the same as for the CAR= 8 nanowires. In doing so, we find in Fig. 9 very good agreement between the modified Jing model and the CAR nanowires with aspect ratios of 6 and 24, even when the nanowire cross section was the smallest considered in the present work, or a=5 nm. This finding suggests that nonlinear elastic effects resulting from the reduced nanowire crosssectional size are not the cause for the difference between the SCB and modified Jing model for the CAR=8 nanowires in Fig. 8, but instead result from the wellknown fact that continuum beam theory loses accuracy for smaller aspect ratios, and due to the neglect of shear deformation for short aspect ratio nanowires in the Jing model
10 GENG YUN AND HAROLD S. PARK PHYSICAL REVIEW B 79, Bending Stiffness of Fixed/Fixed CAR=6 Nanowires SCB Jing:No ν,+c Bending Stiffness of Fixed/Fixed CAR=24 Nanowires SCB Jing:No ν,+c.8 Jing:ν, C 2.8 Jing:ν, C k surf /k bulk k surf /k bulk FIG. 9. Color online Comparison between SCB results and two different Jing models for CAR nanowires where CAR=6 and CAR =24, with same square nanowire crosssectional lengths a as for CAR=8 nanowires discussed earlier. While there is relatively good agreement for fixed/fixed nanowire bending stiffnesses between the SCB results and the Jing analytic results, they are entirely different for the fixed/free case, as illustrated in Fig. for both nanowire geometries considered. In particular, it is observed that while the original Jing linear surfaceelastic analytic solution in Eq. 4 predicts a significant increase in normalized bending stiffness for the fixed/free nanowires, the SCB solution predicts a very slight decrease for both CCSA and CAR geometries. We additionally note that while the modified Jing model reduces the difference as compared to the SCB results, the modified Jing model still predicts that fixed/free nanowires are stiffer than the corresponding bulk material with decreasing nanowire size. We emphasize that recent atomistic calculations for the bending properties of fixed/free silver nanowires with surfaces by McDowell et al. 36 also found an essentially bulk response for nanowires with this boundary condition for crosssectional lengths larger than about 4 nm, while experiments by Petrova et al., 2 Zijlstra et al., 22 and Li et al. 23 on freestanding gold nanowires also showed a slight decrease in the nanowire Young s modulus. We additionally note that in both the Petrova 2 and Zijlstra 22 experimental studies, the nanowires had a axial orientation, similar to the SCB nanowires studied in the present work. The reason why the fixed/free SCB nanowires exhibit different elastic properties under bending than are predicted using the linear Jing surfaceelastic solution in Eq. 4 is as follows. Because of the surface stresses, the free end of the nanowire compresses significantly.6% or more for the 6 nm cross section CCSA nanowires 48, which alters the elastic properties of not only the nonlinearly elastic bulk stiffness, but also the nonlinearly elastic surface stiffness, as the SCB model is a nonlinear, finite deformation constitutive model. In particular, compressive strain is known to lead to elastic softening of bulk FCC metal crystals; 28,29 therefore, the bulkelastic softening which results from the surfacestressdriven contraction clearly mitigates the effects of the tensile surface stress for fixed/free nanowires, leading to the slight overall decrease in elastic stiffness as seen in Fig.. k surf /k bulk Bending Stiffness of Fixed/Free CAR Nanowires SCB Jing:No ν,+c Jing:ν, C k surf /k bulk Bending Stiffness of Fixed/Free CCSA Nanowires, a=6 nm 5 SCB Jing:No ν,+c Jing:ν, C FIG.. Color online Bulk normalized bending stiffness for fixed/free SCB CAR and CCSA nanowires as compared to the analytic surfaceelastic solutions in Eq
11 SURFACE STRESS EFFECTS ON THE BENDING PHYSICAL REVIEW B 79, In contrast, both the original and modified Jing surfaceelastic bending solutions in Eq. 4 neglect two critical points. First, the compressive relaxation strain that is caused by the surface stresses, and which leads to softening of the bulk 28,29 is not accounted for. Second, even if surfacestressdriven compressive strain was captured by Eq. 4, due to the fact that the solutions are based upon linear elasticity, no changes in bulk or surface stiffness due to the deformation would be captured; as seen in Eq. 4, the surface stiffness C is a constant. Therefore, because the Jing solution in Eq. 4 is based upon the linear surfaceelastic theory of Gurtin and Murdoch, 4 and thus depends on both the surface stress, which is generally positive for FCC metals, 59 and the surface stiffness C, which is generally negative for FCC metals, 59 it is realistic as it could possibly predict a decrease in effective modulus due to the presence of the negative surface stiffness C. However, we have shown in the present work that the stiffening effects due to the increase in nanowire length L which results from the L 2 /a 3 term associated with the surface stress in Eq. 4 dominates any softening due to C, and thus a dramatic stiffening is also observed using the Jing solution in Eq. 4 for fixed/free metal nanowires. B. Discussion: Comparison to linear surfaceelastic models based solely on surface energy Because there exists a class of analytic linear surfaceelastic solutions which depend only on the surface energy,,42 and not the surface stress and surface stiffness C, we briefly discuss the implications of the difference form in surfaceelastic solution here. One such solution is that given by Cuenot et al., k scb k bulk =+ 8L2 5ED 3, 5 where D is the diameter of the nanowire assuming a circular cross section. It is easily seen that, since for FCC metals, the Cuenot analytic solution in Eq. 5 can only lead to an increase in Young s modulus with decreasing size. While we also note that Eq. 5 was derived for fixed/fixed nanowires, a similar expression can be derived for fixed/free nanowires, which in contrast to available experimental studies 2 23 and the present SCB results, again guarantees an increase in Young s modulus with decreasing size for fixed/ free nanowires. To further illustrate the importance of nonlinear kinematics in accounting for deformationinduced changes due to surface stresses on the bulk and surface stiffness of nanostructures, we also discuss the analytic solution for nanobeam bending of Guo and Zhao, 42 where relaxation and deformation due to surface stresses are accounted for; however, the surface and bulk constitutive response in that work 42 is linear elastic, so that no changes in material stiffness occur due to the surface stress driven relaxation. In particular, their Eq. 28 gives an expression for the effective Young s modulus accounting for surface relaxation effects as E eff = E bulk + L2 N +2nk 3 a 3, 6 where k is the surface relaxation parameter, which is a positive number chosen to vary between.85 and.5; we note the similarity of this expression to Eq. 5. However, because the surface relaxation parameter k and because the surface energy, the effective Young s modulus described by Eq. 6 must stiffen with decreasing nanowire crosssectional size a for both fixed/fixed and fixed/free boundary conditions. This is again in contrast, for fixed/free boundary conditions, to the SCB results obtained in the present work, recent atomistic simulations, 36 and recent resonant experiments on gold nanowires, 2,22 all of which predict slight decreases in gold nanowire Young s modulus for fixed/free or freestanding boundary conditions. It is worth emphasizing that while previous computational studies of metal nanowires have found a reduced elastic modulus due to surface stress effects, 28,29,5 the present finding that softening of fixed/free nanowires can occur despite the presence of surface stresses has not been found by previous researchers,,,42,44,45 mainly due to the fact that the analytic works have considered fixed/fixed boundary conditions only. The present results strongly indicate that a combination of key factors, including boundary conditions and changes in both surface and bulkelastic properties due to surface stress driven relaxation, must be accounted for to accurately predict the boundaryconditiondependent bendingderived elastic properties of metal nanowires that are subject to surface stresses. C. Discussion: Comparison of nanowire Young s modulus from bending and resonance SCB calculations We conclude our analysis by presenting a comparison between Young s modulus of the metal nanowires as computed in the present work using bending simulations, and SCB resonance simulations of the nanowire Young s modulus as previously described by Park and Klein. 5 An analysis of Young s modulus that might be expected from different loading methods is critical due to the fact that experimentally, bending and resonance of nanowires are the two most common methods to extract, by using continuum beam theory relationships, Young s modulus of the nanowires. For the SCB resonance calculations, we first calculated the resonant frequencies through solution of a standard finite element eigenvalue problem, where the FEM stiffness matrix is the relaxed stiffness matrix after deformation due to surface stresses. After obtaining the resonant frequencies, the nanowire Young s modulus was obtained by relating the resonant frequencies to Young s modulus using standard continuum beam theory expressions. 63 The comparison of the fixed/fixed CCSA and CAR nanowires are shown in Fig.. In all figures, we plot the bulknormalized Young s modulus against the inverse length ratio L 2 /a 3, in accordance with the analytic solutions for bending in Eqs. 3 and 4. As can be seen in Fig., the bulk
12 GENG YUN AND HAROLD S. PARK PHYSICAL REVIEW B 79, E scb /E bulk Modulus Comparison for Fixed/Fixed CCSA Nanowires 2.8 SCB Bending 2.6 SCB Resonance E scb /E bulk Modulus Comparison for Fixed/Fixed CAR Nanowires SCB Bending SCB Resonance FIG.. Color online Comparison of nanowire Young s modulus obtained from SCB bending and resonance calculations for fixed/fixed CCSA and CAR nanowires. normalized Young s modulus for fixed/fixed boundary conditions is found to be nearly identical whether bending or resonance calculations are performed, for both CAR and CCSA nanowires. We show in Fig. 2 the comparison of the bulknormalized Young s modulus for the fixed/free CCSA and CAR nanowires. Again, very little discrepancy between Young s modulus obtained via resonance or via bending is found, where both the SCB bending and resonance calculations predict a very slight decrease in nanowire Young s modulus as compared to the bulk value for both CAR and CCSA geometries. We note again the agreement with recent experimental results showing the same trend for fixed/free or free standing gold nanowires The present results collectively indicate that surface stresses have a similar effect on the elastic properties of nanowires as measured using either resonance or bending testing techniques. VII. CONCLUSIONS In conclusion, we have utilized the surface CauchyBorn model to quantify the effects of surface stresses on the bending behavior and properties of gold nanowires with transverse surfaces. By studying the bending behavior and properties of nanowires accounting for both fixed/fixed and fixed/free boundary conditions, we have found that: in agreement with available experimental data, Young s modulus of the nanowires varies depending on the boundary condition; a distinct stiffening was found for fixed/fixed boundary conditions,, while a very slight softening was found for fixed/free boundary conditions The stresses in the nanowires resulting from surface stressinduced deformation, for both boundary conditions, are significantly larger than the stresses generated through bending unless very large bending strains 5% are reached. 3 The displacements along the nanowire cross section due to surface stress induced deformation are also on the same order as the deformations due to bending unless large % bending strains are generated. 4 Because of the magnitude of the stresses and displacements in the nanowires induced by surface stresses in the absence of applied bending forces, continuum beam theories for bending do not appear to be applicable in describing the stresses and displacements of nanowires. 5 Analytic solutions in the literature that are Modulus Comparison for Fixed/Free CCSA Nanowires.5 SCB Bending SCB Resonance.998 Modulus Comparison for Fixed/Free CAR Nanowires SCB Bending SCB Resonance E scb /E bulk E scb /E bulk FIG. 2. Color online Comparison of nanowire Young s modulus from SCB bending and resonance calculations for fixed/free CCSA and CAR nanowires
This article appeared in a journal published by Elsevier. The attached copy is furnished to the author for internal noncommercial research and
This article appeared in a journal published by Elsevier. The attached copy is furnished to the author for internal noncommercial research and education use, including for instruction at the authors institution
More informationINFLUENCE OF PILES ON LOAD SETTLEMENT BEHAVIOUR OF RAFT FOUNDATION
INFLUENCE OF PILES ON LOAD SETTLEMENT BEHAVIOUR OF RAFT FOUNDATION BALESHWAR SINGH Department of Civil Engineering Indian Institute of Technology Guwahati Guwahati 78139, India NINGOMBAM THOIBA SINGH
More informationFailure of Engineering Materials & Structures. Code 34. Bolted Joint s Relaxation Behavior: A FEA Study. Muhammad Abid and Saad Hussain
Failure of Engineering Materials & Structures Code 3 UET TAXILA MECHNICAL ENGINEERING DEPARTMENT Bolted Joint s Relaxation Behavior: A FEA Study Muhammad Abid and Saad Hussain Faculty of Mechanical Engineering,
More informationRevised zone method Rvalue calculation for precast concrete. sandwich panels containing metal wythe connectors. ByoungJun Lee and Stephen Pessiki
Revised zone method R calculation for precast concrete sandwich panels containing metal wythe connectors ByoungJun Lee and Stephen Pessiki Editor s quick points n Metal wythe connectors are used in a
More informationAnalysis of a Nailed Soil Slope Using Limit Equilibrium and Finite Element Methods
Int. J. of Geosynth. and Ground Eng. (2016) 2:34 DOI 10.1007/s4089101600760 Analysis of a Nailed Soil Slope Using Limit Equilibrium and Finite Element Methods S. Rawat 1 A. K. Gupta 1 Received: 5 September
More informationExperimental investigation of crack in aluminum cantilever beam using vibration monitoring technique
International Journal of Computational Engineering Research Vol, 04 Issue, 4 Experimental investigation of crack in aluminum cantilever beam using vibration monitoring technique 1, Akhilesh Kumar, & 2,
More informationEWGAE 2010 Vienna, 8th to 10th September
EWGAE 2010 Vienna, 8th to 10th September Frequencies and Amplitudes of AE Signals in a Plate as a Function of Source Rise Time M. A. HAMSTAD University of Denver, Department of Mechanical and Materials
More informationAN INNOVATIVE FEA METHODOLOGY FOR MODELING FASTENERS
AN INNOVATIVE FEA METHODOLOGY FOR MODELING FASTENERS MacArthur L. Stewart 1 1 Assistant Professor, Mechanical Engineering Technology Department, Eastern Michigan University, MI, USA Abstract Abstract Researchers
More informationEFFECT OF ADHEREND SHAPE ON STRESS CONCENTRATION REDUCTION OF ADHESIVELY BONDED SINGLE LAP JOINT
Engineering Review, Vol. 36, Issue 1, 2934, 16. 29 EFFECT OF ADHEREND SHAPE ON STRESS CONCENTRATION REDUCTION OF ADHESIVELY BONDED SINGLE LAP JOINT A. Çalık 1* 1 Department of Mechanical Engineering,
More informationNALYSIS OF STABILIZING SLOPES USING VERTICAL PILES
NALYSIS OF STABILIZING SLOPES USING VERTICAL PILES Mahmoud S. Abdelbaki: Lecturer, Gehan E. Abdelrahman: Lecturer, Youssef G. Youssef :Assis.Lecturer, Civil Eng. Dep., Faculty of Eng., Cairo University,
More informationModule 2 WAVE PROPAGATION (Lectures 7 to 9)
Module 2 WAVE PROPAGATION (Lectures 7 to 9) Lecture 9 Topics 2.4 WAVES IN A LAYERED BODY 2.4.1 Onedimensional case: material boundary in an infinite rod 2.4.2 Three dimensional case: inclined waves 2.5
More informationEFFECTS OF LATERAL PLATE DIMENSIONS ON ACOUSTIC EMISSION SIGNALS FROM DIPOLE SOURCES. M. A. HAMSTAD*, A. O'GALLAGHER and J. GARY
EFFECTS OF LATERAL PLATE DIMENSIONS ON ACOUSTIC EMISSION SIGNALS FROM DIPOLE SOURCES ABSTRACT M. A. HAMSTAD*, A. O'GALLAGHER and J. GARY National Institute of Standards and Technology, Boulder, CO 835
More informationResonant Frequency Analysis of the Diaphragm in an Automotive Electric Horn
Resonant Frequency Analysis of the Diaphragm in an Automotive Electric Horn R K Pradeep, S Sriram, S Premnath Department of Mechanical Engineering, PSG College of Technology, Coimbatore, India 641004 Abstract
More informationFINITE ELEMENT MODELLING FOR TENSILE BEHAVIOUR OF THERMALLY BONDED NONWOVEN FABRIC
FINITE ELEMENT MODELLING FOR TENSILE BEHAVIOUR OF THERMALLY BONDED NONWOVEN FABRIC Xiaoping Gao*, Liping Wang Inner Mongolia University of Technology, College of Light Industry and Textile, Hohhot, Inner
More informationFLEXURE STRENGTH AND FAILURE PROBABILITY OF SILICON NANOWIRES
The Pennsylvania State University The Graduate School College of Earth and Mineral Science FLEXURE STRENGTH AND FAILURE PROBABILITY OF SILICON NANOWIRES A Dissertation in Materials Science and Engineering
More informationKorean standards of visual grading and establishing allowable properties of softwood structural lumber
Korean standards of visual grading and establishing allowable properties of softwood structural lumber Park, MoonJae 1, Shim, KugBo 1 ABSTRACT Korean standards related to wood products such as "Sizes
More informationNUMERICAL AND EXPERIMENTAL VALIDATION OF CHIP MORPHOLOGY
International Journal of Advanced Research in Engineering and Technology (IJARET) Volume 10, Issue 2, March April 2019, pp. 503508, Article ID: IJARET_10_02_049 Available online at http://www.iaeme.com/ijaret/issues.asp?jtype=ijaret&vtype=10&itype=02
More informationConsideration of Tool Chamfer for Realistic Application of the Incremental HoleDrilling Method
Consideration of Tool Chamfer for Realistic Application of the Incremental HoleDrilling Method Nicola Simon 1, a *, Jens Gibmeier 1, b 1 Karlsruhe Institute of Technology (KIT), Institute for Applied
More informationEFFECT OF YARN CROSSSECTIONAL SHAPES AND CRIMP ON THE MECHANICAL PROPERTIES OF 3D WOVEN COMPOSITES
EFFECT OF YARN CROSSSECTIONAL SHAPES AND CRIMP ON THE MECHANICAL PROPERTIES OF 3D WOVEN COMPOSITES S. Kari, M. Kumar, I.A. Jones, N.A. Warrior and A.C. Long Division of Materials, Mechanics & Structures,
More informationEFFECTS OF GEOMETRY ON MECHANICAL BEHAVIOR OF DOVETAIL CONNECTION
EFFECTS OF GEOMETRY ON MECHANICAL BEHAVIOR OF DOVETAIL CONNECTION Gi Young Jeong 1, MoonJae Park 2, KweonHwan Hwang 3, JooSaeng Park 2 ABSTRACT: The goal of this study is to analyze the effects of geometric
More information4.0 MECHANICAL TESTS. 4.2 Structural tests of cedar shingles
4.0 MECHANICAL TESTS 4.1 Basis for the test methodology The essence of deterioration is that while it may be caused by insects, weather, fungi or bacteria, the decay is not identical. Further, no two physical
More informationIJSRD  International Journal for Scientific Research & Development Vol. 4, Issue 05, 2016 ISSN (online):
IJSRD  International Journal for Scientific Research & Development Vol. 4, Issue 05, 2016 ISSN (online): 23210613 Static Analysis of VMC Spindle for Maximum Cutting Force Mahesh M. Ghadage 1 Prof. Anurag
More informationANALYSIS OF LATERAL STIFFNESS FOR INFILLED FRAME WITH OPENING
ANALYSIS OF LATERAL STIFFNESS FOR INFILLED FRAME WITH OPENING A.S. KASNALE 1 & SANJAY JAMKAR 2 Professor in Civil Engineering Department, M.S. Bidve Engineering College, Latur, India Professor in Civil
More informationCHAPTER 6 CARBON NANOTUBE AND ITS RF APPLICATION
CHAPTER 6 CARBON NANOTUBE AND ITS RF APPLICATION 6.1 Introduction In this chapter we have made a theoretical study about carbon nanotubes electrical properties and their utility in antenna applications.
More informationINFLUENCE OF SOME MODIFICATIONS OF LOCAL GEOMETRY ON THE STRESS STATES IN ADHESIVE BONDED LAP JOINTS
SISOM 2009 and Session of the Commission of Acoustics, Bucharest 2829 May INFLUENCE OF SOME MODIFICATIONS OF LOCAL GEOMETRY ON THE STRESS STATES IN ADHESIVE BONDED LAP JOINTS Adriana SANDU *, Marin SANDU
More informationNonlinear behavior of Reinforced Concrete Infilled Frames using ATENA 2D
Available online at www.ijacskros.com Indian Journal of Advances in Chemical Science S1 (2016) 173178 Nonlinear behavior of Reinforced Concrete Infilled Frames using ATENA 2D M. D. Raghavendra Prasad,
More informationTORQUE DESIGN, ANALYSIS AND CHARACTERIZATION OF CRITICAL FASTENERS IN DIESEL ENGINES
TORQUE DESIGN, ANALYSIS AND CHARACTERIZATION OF CRITICAL FASTENERS IN DIESEL ENGINES ROHIT PATIL 1, MUKUND NALAWADE 2, NITIN GOKHALE 3. 1 P.G. Student, Department of Mechanical Engineering, Vishwakarma
More information3D Finite Element Analysis of Bolted Joint Using Helical Thread Model
3D Finite Element Analysis of Bolted Joint Using Helical Thread Model Shaik Gousia Yasmin 1, P. Punna Rao 2, Kondaiah Bommisetty 3 1 M.Tech(CAD/CAM), Nimra College of Engineering & Technology, Vijayawada,
More informationFINITE ELEMENT SIMULATIONS OF THE EFFECT OF FRICTION COEFFICIENT IN FRETTING WEAR
Proceedings of the 5 th International Conference on Fracture Fatigue and Wear, pp. 5863, 216 FINITE ELEMENT SIMULATIONS OF THE EFFECT OF FRICTION COEFFICIENT IN FRETTING WEAR T. Yue and M. Abdel Wahab
More informationInvestigating Mechanical Properties of Metallic Nanowires using Molecular Dynamics
Virginia Commonwealth University VCU Scholars Compass Theses and Dissertations Graduate School 2014 Investigating Mechanical Properties of Metallic Nanowires using Molecular Dynamics Alex Khammang Virginia
More informationFinite Element Analysis of MultiFastened Bolted Joint Connecting Composite Components in Aircraft Structures
Finite Element Analysis of MultiFastened Bolted Joint Connecting Composite Components in Aircraft Structures Dr. M Satyanarayana Gupta Professor & HoD, Dept. of Aeronautical Engineering MLRIT, Hyderabad.
More informationDowel connections in laminated strand lumber
Dowel connections in laminated strand lumber Cranswick, Chad J. 1, M c Gregor, Stuart I. 2 ABSTRACT Laminated strand lumber (LSL) is a relatively new structural composite lumber. As such, very limited
More informationElectronic Noise Effects on Fundamental LambMode Acoustic Emission Signal Arrival Times Determined Using Wavelet Transform Results
DGZfPProceedings BB 9CD Lecture 62 EWGAE 24 Electronic Noise Effects on Fundamental LambMode Acoustic Emission Signal Arrival Times Determined Using Wavelet Transform Results Marvin A. Hamstad University
More informationMODEL MODIFICATION OF WIRA CENTER MEMBER BAR
MODEL MODIFICATION OF WIRA CENTER MEMBER BAR F.R.M. Romlay & M.S.M. Sani Faculty of Mechanical Engineering Kolej Universiti Kejuruteraan & Teknologi Malaysia (KUKTEM), Karung Berkunci 12 25000 Kuantan
More informationFastener Modeling for Joining Parts Modeled by Shell and Solid Elements
200708 Fastener Modeling for Joining Parts Modeled by Shell and Solid Elements Aleander Rutman, Chris Boshers Spirit AeroSystems Larry Pearce, John Parady MSC.Software Corporation 2007 Americas Virtual
More informationFigure 1 : Topologies of a capacitive switch The actuation voltage can be expressed as the following :
ABSTRACT This paper outlines the issues related to RF MEMS packaging and low actuation voltage. An original approach is presented concerning the modeling of capacitive contacts using multiphysics simulation
More informationEXPERIMENTAL ANALYSIS OF BOLT LOOSENING DYNAMICS CHARACTERISTIC IN A BEAM BY IMPACT TESTING
EXPERIMENTAL ANALYSIS OF BOLT LOOSENING DYNAMICS CHARACTERISTIC IN A BEAM BY IMPACT TESTING Meifal Rusli, Candra Mardianto and Mulyadi Bur Department of Mechanical Engineering, Faculty of Engineering,
More informationQuantitative Crack Depth Study in Homogeneous Plates Using Simulated Lamb Waves.
More Info at Open Access Database www.ndt.net/?id=18675 Quantitative Crack Depth Study in Homogeneous Plates Using Simulated Lamb Waves. Mohammad. (. SOORGEE, Aghil. YOUSEF)KOMA Nondestructive Testing
More information3D NonLinear FEA to Determine Burst and Collapse Capacity of Eccentrically Worn Casing
3D NonLinear FEA to Determine Burst and Collapse Capacity of Eccentrically Worn Casing Mark Haning Asst. Prof James Doherty Civil and Resource Engineering, University of Western Australia Andrew House
More informationStress Analysis of Flanged Joint Using Finite Element Method
Stress Analysis of Flanged Joint Using Finite Element Method Shivaji G. Chavan Assistant Professor, Mechanical Engineering Department, Finolex Academy of Management and Technology, Ratnagiri, Maharashtra,
More informationSettlement Analysis of Piled Raft System in Soft Stratified Soils
Settlement Analysis of Piled Raft System in Soft Stratified Soils Srinivasa Reddy Ayuluri 1, Dr. M. Kameswara Rao 2 1 (PG Scholar, Civil Engineering Department, Malla Reddy Engineering College, Hyderabad,
More informationEFFECT OF HOLE CLEARANCE ON BOLT LOADS IN PULTRUDED GRP TENSION JOINTS
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EFFECT OF HOLE CLEARANCE ON BOLT LOADS IN PULTRUDED GRP TENSION JOINTS Geoffrey J Turvey*, Pu Wang** *Lancaster University, **Schlumberger Keywords:
More informationVIBRATIONAL TESTING OF A FULLSCALE PILE GROUP IN SOFT CLAY
VIBRATIONAL TESTING OF A FULLSCALE PILE GROUP IN SOFT CLAY Marvin W HALLING 1, Kevin C WOMACK 2, Ikhsan MUHAMMAD 3 And Kyle M ROLLINS 4 SUMMARY A 3 x 3 pile group and pile cap were constructed in a soft
More informationModeling MultiBolted Systems
Modeling MultiBolted Systems Jerome Montgomery Siemens Power Generation Abstract Modeling a single bolt in a finite element analysis raises questions of how much complexity to include. But, modeling a
More informationPRACTICAL ASPECTS OF ACOUSTIC EMISSION SOURCE LOCATION BY A WAVELET TRANSFORM
PRACTICAL ASPECTS OF ACOUSTIC EMISSION SOURCE LOCATION BY A WAVELET TRANSFORM Abstract M. A. HAMSTAD 1,2, K. S. DOWNS 3 and A. O GALLAGHER 1 1 National Institute of Standards and Technology, Materials
More informationGEOMETRIC MODELING OF WIRE ROPE
International Journal of Technical Innovation in Modern Engineering & Science (IJTIMES) Impact Factor: 5.22 (SJIF217), eissn: 24552585 Volume 4, Issue 8, August218 GEOMETRIC MODELING OF WIRE ROPE Krishan
More informationSupplementary information for Stretchable photonic crystal cavity with
Supplementary information for Stretchable photonic crystal cavity with wide frequency tunability Chun L. Yu, 1,, Hyunwoo Kim, 1, Nathalie de Leon, 1,2 Ian W. Frank, 3 Jacob T. Robinson, 1,! Murray McCutcheon,
More informationCHAPTER 2 ELECTROMAGNETIC FORCE AND DEFORMATION
18 CHAPTER 2 ELECTROMAGNETIC FORCE AND DEFORMATION 2.1 INTRODUCTION Transformers are subjected to a variety of electrical, mechanical and thermal stresses during normal life time and they fail when these
More informationModel Correlation of Dynamic Nonlinear Bearing Behavior in a Generator
Model Correlation of Dynamic Nonlinear Bearing Behavior in a Generator Dean Ford, Greg Holbrook, Steve Shields and Kevin Whitacre Delphi Automotive Systems, Energy & Chassis Systems Abstract Efforts to
More informationModal Analysis of Microcantilever using Vibration Speaker
Modal Analysis of Microcantilever using Vibration Speaker M SATTHIYARAJU* 1, T RAMESH 2 1 Research Scholar, 2 Assistant Professor Department of Mechanical Engineering, National Institute of Technology,
More informationMonopile as Part of Aeroelastic Wind Turbine Simulation Code
Monopile as Part of Aeroelastic Wind Turbine Simulation Code Rune Rubak and Jørgen Thirstrup Petersen Siemens Wind Power A/S Borupvej 16 DK7330 Brande Denmark Abstract The influence on wind turbine design
More informationChapter  6. Aluminium Alloy AA6061. The alloy is of intermediate strength but possesses excellent
107 Chapter  6 Aluminium Alloy AA6061 The alloy is of intermediate strength but possesses excellent corrosion resistance and has high plane strain fracture toughness. It is readily welded. Typical applications
More informationVoid Reduction in Reflow Soldering Processes by Sweep Stimulation of PCB Substrate
Void Reduction in Reflow Soldering Processes by Sweep Stimulation of PCB Substrate Viktoria Rawinski Ersa GmbH Wertheim, Germany Abstract Due to the ongoing trend towards miniaturization of power components,
More informationGENERAL GUIDELINES FOR APPLICATION OF THE EXTENDED SUBTRACTION METHOD IN SASSI SOILSTRUCTURE INTERACTION ANALYSIS
Transactions, SMiRT22 GENERAL GUIDELINES FOR APPLICATION OF THE EXTENDED SUBTRACTION METHOD IN SASSI SOILSTRUCTURE INTERACTION ANALYSIS C. C. Chin 1, Nan Deng 2, and Farhang Ostadan 3 1 Senior Engineer,
More informationShould We Upgrade to Phase 2 6.0?
Should We Upgrade to Phase 2 6.0? Rocscience has released version 6.0 of Phase 2, the popular twodimensional finite element program for analyzing and designing surface and underground excavations in rock
More informationInvestigating the Electronic Behavior of Nanomaterials From Charge Transport Properties to System Response
Investigating the Electronic Behavior of Nanomaterials From Charge Transport Properties to System Response Amit Verma Assistant Professor Department of Electrical Engineering & Computer Science Texas
More informationDynamic Modeling of Air Cushion Vehicles
Proceedings of IMECE 27 27 ASME International Mechanical Engineering Congress Seattle, Washington, November 5, 27 IMECE 274 Dynamic Modeling of Air Cushion Vehicles M Pollack / Applied Physical Sciences
More informationEfficient Electromagnetic Analysis of Spiral Inductor Patterned Ground Shields
Efficient Electromagnetic Analysis of Spiral Inductor Patterned Ground Shields James C. Rautio, James D. Merrill, and Michael J. Kobasa Sonnet Software, North Syracuse, NY, 13212, USA Abstract Patterned
More informationAn Investigation of Optimal Pitch Selection to Reduce SelfLoosening of Threaded Fastener under Transverse Loading
IJSTE  International Journal of Science Technology & Engineering Volume 3 Issue 01 July 2016 ISSN (online): 2349784X An Investigation of Optimal Pitch Selection to Reduce SelfLoosening of Threaded Fastener
More informationTHE INFLUENCE OF GOUGE DEFECTS ON FAILURE PRESSURE OF STEEL PIPES
International Conference on Mechanical Engineering Research (ICMER2013), 13 July 2013 Bukit Gambang Resort City, Kuantan, Pahang, Malaysia Organized by Faculty of Mechanical Engineering, Universiti Malaysia
More informationEnhancing the low frequency vibration reduction performance of plates with embedded Acoustic Black Holes
Enhancing the low frequency vibration reduction performance of plates with embedded Acoustic Black Holes Stephen C. CONLON 1 ; John B. FAHNLINE 1 ; Fabio SEMPERLOTTI ; Philip A. FEURTADO 1 1 Applied Research
More informationThe influence of gouge defects on failure pressure of steel pipes
IOP Conference Series: Materials Science and Engineering OPEN ACCESS The influence of gouge defects on failure pressure of steel pipes To cite this article: N A Alang et al 2013 IOP Conf. Ser.: Mater.
More informationNumerical Modeling of Grouted Soil Nails
Numerical Modeling of Grouted Soil Nails Dr. Haider S. Al Jubair Department of Civil Engineering University of BasrahCollege of Engineering Basrah, Iraq Afaf A. Maki Department of Civil Engineering University
More informationCHAPTER 3 SHORT CIRCUIT WITHSTAND CAPABILITY OF POWER TRANSFORMERS
38 CHAPTER 3 SHORT CIRCUIT WITHSTAND CAPABILITY OF POWER TRANSFORMERS 3.1 INTRODUCTION Addition of more generating capacity and interconnections to meet the ever increasing power demand are resulted in
More informationPreliminary study of the vibration displacement measurement by using strain gauge
Songklanakarin J. Sci. Technol. 32 (5), 453459, Sep.  Oct. 2010 Original Article Preliminary study of the vibration displacement measurement by using strain gauge Siripong Eamchaimongkol* Department
More informationLoughborough University Institutional Repository. This item was submitted to Loughborough University's Institutional Repository by the/an author.
Loughborough University Institutional Repository Finite element simulation of lowdensity thermally bonded nonwoven materials: effects of orientation distribution function and arrangement of bond points
More informationInspection of pipe networks containing bends using long range guided waves
Inspection of pipe networks containing bends using long range guided waves Ruth Sanderson TWI Ltd. Granta Park, Great Abington, Cambridge, CB21 6AL, UK 1223 899 ruth.sanderson@twi.co.uk Abstract Guided
More informationModelling of Rebar and Cable Bolt Behaviour in Tension/Shear
University of Wollongong Research Online Coal Operators' Conference Faculty of Engineering and Information Sciences 2015 Modelling of Rebar and Cable Bolt Behaviour in Tension/Shear Xuwei Li University
More informationA Study on Effect of Sizing Bolt Hole in SingleLap Connection Using FEA
Journal of Scientific Research & Reports 19(1): 114, 2018; Article no.jsrr.40498 ISSN: 23200227 A Study on Effect of Sizing Bolt Hole in SingleLap Connection Using FEA Anil Zafer 1, Orkun Yilmaz 1*
More informationComparison of FRD (Focal Ratio Degradation) for Optical Fibres with Different Core Sizes By Neil Barrie
Comparison of FRD (Focal Ratio Degradation) for Optical Fibres with Different Core Sizes By Neil Barrie Introduction The purpose of this experimental investigation was to determine whether there is a dependence
More informationAcoustic Emission Signals versus Propagation Direction for Hybrid Composite Layup with Large Stiffness Differences versus Direction
31 st Conference of the European Working Group on Acoustic Emission (EWGAE) We.1.A.1 More Info at Open Access Database www.ndt.net/?id=17568 Acoustic Emission Signals versus Propagation Direction for Hybrid
More informationLORENTZ FORCE DETUNING ANALYSIS OF THE SPALLATION NEUTRON SOURCE (SNS) ACCELERATING CAVITIES *
LORENTZ FORCE DETUNING ANALYSIS OF THE SPALLATION NEUTRON SOURCE (SNS) ACCELERATING CAVITIES * R. Mitchell, K. Matsumoto, Los Alamos National Lab, Los Alamos, NM 87545, USA G. Ciovati, K. Davis, K. Macha,
More informationwhich arise due to finite size, can be useful for efficient energy transfer away from the drive
C h a p t e r 7 87 WEAKLY NONLINEAR DYNAMIC REGIME: NONLINEAR RESONANCES AND ENERGY TRANSFER IN FINITE GRANULAR CHAINS Abstract In the present work we test experimentally and compute numerically the stability
More informationModal vibration control of submarine hulls
Modal vibration control of submarine hulls B. Alzahabi Department of Mechanical Engineering, Kettering University, USA Abstract Cylindrical shells are widely used in many structural designs, such as offshore
More informationDrawing of Hexagonal Shapes from Cylindrical Cups
Dr. Waleed Khalid Jawed Metallurgy & Production Engineering Department, University of Technology /Baghdad Email: Drwaleed555@yahoo.com Sabih Salman Dawood Metallurgy & Production Engineering Department,
More informationarxiv: v3 [condmat.mtrlsci] 17 Dec 2015
Highly Stretchable MoS 2 Kirigami Paul Z. Hanakata and David K. Campbell Department of Physics, Boston University, Boston, MA 2215, USA Zenan Qi and Harold S. Park Department of Mechanical Engineering,
More informationComparing the State Estimates of a Kalman Filter to a Perfect IMM Against a Maneuvering Target
14th International Conference on Information Fusion Chicago, Illinois, USA, July 8, 11 Comparing the State Estimates of a Kalman Filter to a Perfect IMM Against a Maneuvering Target Mark Silbert and Core
More informationAbaqus Beam Tutorial (ver. 6.12)
Abaqus Beam Tutorial (ver. 6.12) Problem Description The twodimensional bridge structure is simply supported at its lower corners. The structure is composed of steel Tsections (E = 210 GPa, ν = 0.25)
More informationNumerical Analysis of Piled Raft Foundation using Fem with Interaction Effects
International Journal of TechnoChem Research ISSN:23954248 www.technochemsai.com Vol.01, No.03, pp 126134, 2015 Numerical Analysis of Piled Raft Foundation using Fem with Interaction Effects Naveen kumar.d
More informationWITHDRAWAL AND LATERAL STRENGTH OF THREADED NAILS
238 WITHDRAWAL AND LATERAL STRENGTH OF THREADED NAILS Douglas R. Rammer, Donald A. Bender, and David G. Pollock An experimental study on the performance of threaded nails was conducted to understand and
More informationOptimizing the Natural Frequencies of Beams via Notch Stamping
Research Journal of Applied Sciences, Engineering and Technology 4(14): 20302035, 2012 ISSN: 20407467 Maxwell Scientific Organization, 2012 Submitted: December 02, 2011 Accepted: December 26, 2011 Published:
More informationExperimental Investigation of Crack Detection in Cantilever Beam Using Natural Frequency as Basic Criterion
INSTITUTE OF TECHNOLOGY, NIRMA UNIVERSITY, AHMEDABAD 382 481, 0810 DECEMBER, 2011 1 Experimental Investigation of Crack Detection in Cantilever Beam Using Natural Frequency as Basic Criterion A. A.V.Deokar,
More informationROBUST PARAMETER DESIGN AND FINITE ELEMENT ANALYSIS FOR A NON PNEUMATIC TIRE WITH LOW VIBRATION
Clemson University TigerPrints All Theses Theses 122009 ROBUST PARAMETER DESIGN AND FINITE ELEMENT ANALYSIS FOR A NON PNEUMATIC TIRE WITH LOW VIBRATION Amarnath Proddaturi Clemson University, aprodda@clemson.edu
More informationAcoustic Resonance Analysis Using FEM and Laser Scanning For Defect Characterization in InProcess NDT
ECNDT 2006  We.4.8.1 Acoustic Resonance Analysis Using FEM and Laser Scanning For Defect Characterization in InProcess NDT Ingolf HERTLIN, RTE Akustik + Prüftechnik, Pfinztal, Germany Abstract. This
More informationModelling III ABSTRACT
Modelling III Hybrid FEVIM Model of Eddy Current Inspection of Steam Generator Tubes in the Vicinity of Tube Support Plates S. Paillard, A. Skarlatos, G. Pichenot, CEA LIST, France G. Cattiaux, T. Sollier,
More informationLaboratory 1: Uncertainty Analysis
University of Alabama Department of Physics and Astronomy PH101 / LeClair May 26, 2014 Laboratory 1: Uncertainty Analysis Hypothesis: A statistical analysis including both mean and standard deviation can
More informationFinite Element Study of Using Concrete Tie Beams to Reduce Differential Settlement Between Footings
Finite Element Study of Using Concrete Tie Beams to Reduce Differential Settlement Between Footings AMIN H. ALMASRI* AND ZIAD N. TAQIEDDIN** *Assistant Professor, Department of Civil Engineering, Jordan
More informationNUMERICAL ANALYSIS OF SCREW ANCHOR FOR CONCRETE
VIII International Conference on Fracture Mechanics of Concrete and Concrete Structures FraMCoS8 J.G.M. Van Mier, G. Ruiz, C. Andrade, R.C. Yu and X.X. Zhang (Eds) NUMERICAL ANALYSIS OF SCREW ANCHOR FOR
More informationStrain Gauge Measurement A Tutorial
Application Note 078 Strain Gauge Measurement A Tutorial What is Strain? Strain is the amount of deformation of a body due to an applied force. More specifically, strain (ε) is defined as the fractional
More informationThermal Cycling and Fatigue
Thermal Cycling and Fatigue Gil Sharon Introduction The majority of electronic failures are thermomechanically related by thermally induced stresses and strains. The excessive difference in coefficients
More informationDESIGN EQUATION FOR MULTIPLE FASTENER WOOD CONNECTIONS
DESIGN EQUATION FOR MULTIPLE FASTENER WOOD CONNECTIONS By John J. Zahn, 1 Member, ASCE ABSTRACT: A compared design equation is presented for the design of multiple fastener connections of wood members.
More informationStructural Strength of Lapped ColdFormed Steel ZShaped Purlin Connections with Vertical Slotted Holes
Missouri University of Science and Technology Scholars' Mine International Specialty Conference on Cold Formed Steel Structures (2014)  22nd International Specialty Conference on ColdFormed Steel Structures
More informationModeling and Finite Element Analysis Methods for the Dynamic Crushing of Honeycomb Cellular MesoStructures
Clemson University TigerPrints All Theses Theses 52011 Modeling and Finite Element Analysis Methods for the Dynamic Crushing of Honeycomb Cellular MesoStructures Jesse Schultz Clemson University, jesses@clemson.edu
More informationChapter 3 Broadside Twin Elements 3.1 Introduction
Chapter 3 Broadside Twin Elements 3. Introduction The focus of this chapter is on the use of planar, electrically thick grounded substrates for printed antennas. A serious problem with these substrates
More informationHighspeed wavefront control using MEMS micromirrors T. G. Bifano and J. B. Stewart, Boston University [ ] Introduction
Highspeed wavefront control using MEMS micromirrors T. G. Bifano and J. B. Stewart, Boston University [589527] Introduction Various deformable mirrors for highspeed wavefront control have been demonstrated
More informationStudies on free vibration of FRP aircraft Instruments panel boards
89 Studies on free vibration of FRP aircraft Instruments panel boards E. Chandrasekaran Professor in Dept. of Civil Engineering, Crescent Engineering College 648 India. email: sekharan@vsnl.net and K.
More informationPresented at the 109th Convention 2000 September Los Angeles, California, USA
Development of a PiezoElectric Super Tweeter Suitable for DVDAudio 5 Mitsukazu Kuze and Kazue Satoh Multimedia Development Center Matsushita Electric Industrial Co., Ltd. Kadomacity, Osaka 57 l8, Japan
More informationSImulation of MONopile installation  JIP SIMON
SImulation of MONopile installation  JIP SIMON Ahmed Elkadi Deltares 14 February 2019 MOTIVATION Vanbeekimages.com 14 februari 2019 Matchmaking Day 2019 2 Global substructure statistics/trends 2016 Offshore
More informationMODELLING OF CONCRETE PAVEMENT DOWELSLAB INTERACTION
4 e Conférence spécialisée en génie des transports de la Société canadienne de génie civil 4 th Transportation Specialty Conference of the Canadian Society for Civil Engineering Montréal, Québec, Canada
More informationPart 2: Second order systems: cantilever response
 cantilever response slide 1 Part 2: Second order systems: cantilever response Goals: Understand the behavior and how to characterize second order measurement systems Learn how to operate: function generator,
More information